- Nano Express
- Open Access
Efficient Optical Reflection Modulation by Coupling Interband Transition of Graphene to Magnetic Resonance in Metamaterials
Nanoscale Research Letters volume 14, Article number: 391 (2019)
Designing powerful electromagnetic wave modulators is required for the advancement of optical communication technology. In this work, we study how to efficiently modulate the amplitude of electromagnetic waves in near-infrared region, by the interactions between the interband transition of graphene and the magnetic dipole resonance in metamaterials. The reflection spectra of metamaterials could be significantly reduced in the wavelength range below the interband transition, because the enhanced electromagnetic fields from the magnetic dipole resonance greatly increase the light absorption in graphene. The maximum modulation depth of reflection spectra can reach to about 40% near the resonance wavelength of magnetic dipole, for the interband transition to approach the magnetic dipole resonance, when an external voltage is applied to change the Fermi energy of graphene.
Dynamically controlling the spectral properties of electromagnetic waves by external stimuli such as mechanical force, temperature change, electrical voltage, and laser beam [1,2,3,4] has been drawing increasing interest, because of many applications in the fields of holographic display technology, high-performance sensing, and optical communications. In the past few years, much effort has been made to actively manipulate the transmission, reflection, or absorption spectra of electromagnetic waves, which is based on electrically tunable surface conductivity of graphene, in a very wide frequency range including microwave [5, 6], terahertz (THz) [7,8,9,10,11,12,13,14,15,16,17,18,19,20,21,22,23,24,25,26,27,28,29,30,31,32,33], infrared [34,35,36,37,38,39,40,41,42,43,44,45,46,47,48,49,50,51,52,53,54,55,56,57,58,59,60,61,62,63,64,65], and visible regime [66,67,68,69]. Such graphene-based active manipulation of electromagnetic waves is under external electrical stimulus without re-building-related structures, which aims to efficiently modulate the amplitude [5, 7,8,9,10,11,12,13,14,15,16,17,18,19,20,21, 34,35,36,37,38,39,40,41,42,43,44,45,46,47,48,49,50,51,52,53,54,55,56,57, 66,67,68,69,70,71,72], phase [6, 22,23,24,25,26,27,28, 58,59,60,61,62], and polarization [29,30,31,32,33, 63,64,65] of electromagnetic waves. The three kinds of electromagnetic wave modulators are the most important for signal processing in free-space optical communications [1,2,3,4]. In the far-infrared and THz regime, the surface conductivity of graphene only comprises the contribution of intraband, and graphene has an effective dielectric function that can be described with the standard Drude model . Therefore, at lower frequencies, very similar to noble metals (e.g., Ag and Au), nanostructured graphene is also able to support localized or delocalized surface plasmon resonances  with great electromagnetic field enhancement, which has been widely employed to strengthen light-mater interactions for efficient modulation of electromagnetic waves. For example, in 2012, Sensale-Rodriguez et al. theoretically presented reflectance modulators with an excellent performance at THz frequency, by taking advantage of plasmonic effects in graphene micro-ribbons . In the visible and near-infrared regime, interband contribution dominates the surface conductivity of graphene, whose complex permittivity has a real part of positive value. So, at higher frequencies, graphene itself no longer supports surface plasmon resonances, but behaves more like an ultra-thin dielectric film when it interacts with light. In this situation, various high-quality resonance modes supported in other nanostructured materials are often explored to electrically modulate electromagnetic waves, with the help of the gate-controlled Fermi energy of graphene. For example, Yu et al. studied in theory the amplitude modulation of visible light with graphene, by utilizing Fabry-Perot interference, Mie modes in dielectric nanospheres with a high refractive index, and surface lattice resonances in a periodic array of metal nanoparticles . In past decade, magnetic resonance in metamaterials has been studied extensively and intensively to achieve perfect absorbers of electromagnetic waves [74,75,76,77,78]. However, up to now, there are only a few studies on optical modulators that are based on magnetic resonance in metamaterials with an inserted graphene monolayer .
We will propose an efficient method to modulate the reflection spectra of electromagnetic waves in near-infrared region, by coupling the interband transition of graphene to the magnetic dipole resonance in metamaterials. It is found that the reflection spectra of metamaterials can be largely reduced in the wavelength range below the interband transition of graphene, because the enhanced electromagnetic fields from the magnetic dipole resonance greatly increase the light absorption in graphene. The maximum modulation depth of reflection amplitude can reach to about 40% near the resonance wavelength of magnetic dipole, for the interband transition to be close to the magnetic dipole resonance, when an external voltage is applied to change the Fermi energy of graphene.
We schematically show in Fig. 1 the building block of investigated metamaterials for efficient reflection modulation in near-infrared region, through the interactions between the magnetic dipole resonance and the interband transition of graphene. We carry out numerical calculations by the commercial software package “EastFDTD” [79, 80]. The silica layer has a refractive index of 1.45, and the silver nanostrips and substrate have an experimental dielectric function . The graphene has a relative permittivity calculated by the following formula :
where σintra and σinter are the intraband and interband terms of the surface conductivity of graphene, τ is the electron-phonon relaxation time, Ef is the Fermi energy, and tg is the graphene thickness. The studied metamaterials could be realized in experiment with the help of advanced nanofabrication technology . Firstly, the silver substrate and the silica layer are prepared by thermal evaporation. Then, the monolayer graphene is coated on the silica surface through chemical vapor deposition. Finally, the periodic array of silver nanostrips is fabricated by electron beam lithography.
Results and Discussion
We first discuss the reflection spectra of metamaterials without graphene, as shown by the black line and squares in Fig. 2a. A broad reflection dip at 1210 nm is observed, which is related to a magnetic dipole. When graphene is inserted into metamaterials, the reflection is largely reduced for the wavelengths smaller than 1150 nm (the position of interband transition in graphene), as shown by the red line and circles in Fig. 2a. The reason is that the enhanced electromagnetic fields from the resonance excitation of magnetic dipole hugely increase the light absorption of graphene. Correspondingly, the graphene-induced modulation depth of reflection spectra will gradually increase from about 11 to 28%, when the light wavelength is increased from 1000 nm to the interband transition position, as exhibited in Fig. 2b. The modulation depth is generally defined as (R-R0)/R0, where R and R0 are the reflection spectra with and without graphene inserted in metamaterials .
To demonstrate that the broad reflection dip is relevant to a magnetic dipole, in Fig. 3, we plot the electromagnetic fields on the xoz plane at the wavelength of 1210 nm. The electric fields are mainly distributed around the edges of silver nanostrips, and the magnetic fields are largely localized into the silica region under the silver nanostrips. The field distribution is the typical property of a magnetic dipole resonance . Between the silver substrate and individual nanostrip, the plasmonic near-field hybridization produces anti-parallel currents, as indicated by two black arrows in Fig. 3b. The anti-parallel currents can induce a magnetic moment M counteracting the incident magnetic field to form the magnetic dipole resonance. The resonant wavelength depends strongly on the width w of the silver nanostrips, which will have an obvious red-shift when w is increased.
The position of interband transition can be conveniently tuned when an external voltage is applied to change Fermi energy Ef. The position tunability of interband transition is very helpful to efficiently control the reflection spectra. For Ef to increase from 0.46 to 0.58 eV, the interband transition blue-shifts quickly, as exhibited by the opened circles in Fig. 4a. Simultaneously, the reflection is reduced noticeably in the wavelength range blow the interband transition. Near the resonance wavelength of magnetic dipole, the reflection is reduced to a minimum of about 0.55, when the interband transition is tuned gradually to be across the broadband magnetic dipole. Figure 4b shows the graphene-induced reflection modulation effect for different Ef. With decreasing Ef, the modulation depth of reflection spectra becomes larger and has a maximum of nearly 40% when Ef = 0.46 eV. Furthermore, the tunable wavelength range also becomes much broader, because of the continuous red-shift of interband transition when Ef is decreased. However, in the wavelength range over the interband transition, the reflection spectra are not modulated as compared with the case of no graphene, and so, the modulation depth is almost zero.
The interband transition is closely related to Fermi energy Ef, which can be fully manifested as a sharp spectral feature in the permittivity εg of graphene. In Fig. 5, we give the real and imaginary parts of εg for different Ef. For each Ef, there exists a narrow peak in the real part of εg, and correspondingly an abrupt drop appears in the imaginary part of εg. With decreasing Ef, such a sharp spectral feature red-shifts obviously. In the wavelength range on the right side of the abrupt drop, the imaginary part of εg is very small. This is why the reflection spectra are not modulated for the wavelengths over the interband transition. The position dependence of interband transition on Fermi energy Ef is shown in Fig. 6. We can clearly see that the peak positions of the real part of εg are in excellent agreement with those indicated by the opened circles in Fig. 4a.
We have numerically demonstrated a method to efficiently modulate the reflection spectra of electromagnetic waves in near-infrared region, by coupling the interband transition of graphene to the magnetic dipole resonance in metamaterials. It is found that the reflection spectra can be largely reduced in the wavelength range below the interband transition of graphene, because the enhanced electromagnetic fields from the magnetic dipole resonance greatly increase the light absorption in graphene. The maximum modulation depth of reflection spectra can reach to about 40% near the resonance wavelength of magnetic dipole, for the interband transition to be near the magnetic dipole resonance, when an external voltage is applied to change the Fermi energy of graphene. The reflection modulation effect presented in this work may find potential applications in optical communication systems.
Availability of Data and Materials
All data are fully available without restriction.
Ou JY, Plum E, Zhang JF, Zheludev NI (2013) An electromechanically reconfigurable plasmonic metamaterial operating in the near-infrared. Nat Nanotechnol 8:252–255
Rahm M, Li JS, Padilla WJ (2013) THz wave modulators: a brief review on different modulation techniques. J Infrared Milli Terahz Waves 34:1–27
Hashemi MR, Cakmakyapan S, Jarrahi M (2017) Reconfigurable metamaterials for terahertz wave manipulation. Rep Prog Phys 80:094501
Cheng JR, Fan F, Chang SJ (2019) Recent progress on graphene-functionalized metasurfaces for tunable phase and polarization control. Nanomaterials 9:398
Balci O, Polat EO, Kakenov N, Kocabas C (2015) Graphene-enabled electrically switchable radar-absorbing surfaces. Nat Commun 6:6628
Balci O, Kakenov N, Kocabas C (2017) Controlling phase of microwaves with active graphene surfaces. Appl Phys Lett 110:161102
Liu XD, Chen ZF, Parrott EPJ, Ung BSY, Xu JB, Pickwell-MacPherson E (2017) Graphene based terahertz light modulator in total internal reflection geometry. Adv Opt Mater 5:1600697
Kim TT, Kim H, Kenney M, Park HS, Kim HD, Min B, Zhang S (2018) Amplitude modulation of anomalously refracted terahertz waves with gated-graphene metasurfaces. Adv Opt Mater 6:1700507
Sensale-Rodriguez B, Yan RS, Zhu MD, Jena D, Liu L, Xing HG (2012) Efficient terahertz electro-absorption modulation employing graphene plasmonic structures. Appl Phys Lett 101:261115
Jessop DS, Kindness SJ, Xiao L, Braeuninger-Weimer P, Lin H, Ren Y, Ren CX, Hofmann S, Zeitler JA, Beere HE, Ritchie DA, Degl’Innocenti R (2016) Graphene based plasmonic terahertz amplitude modulator operating above 100 MHz. Appl Phys Lett 108:171101
He XY (2015) Tunable terahertz graphene metamaterials. Carbon 82:229–237
Li Q, Tian Z, Zhang XQ, Singh RJ, Du LL, Gu JQ, Han JG, Zhang WL (2015) Active graphene-silicon hybrid diode for terahertz waves. Nat Commun 6:7082
Liu PQ, Luxmoore IJ, Mikhailov SA, Savostianova NA, Valmorra F, Faist J, Nash GR (2015) Highly tunable hybrid metamaterials employing split-ring resonators strongly coupled to graphene surface plasmons. Nat Commun 6:8969
Sensale-Rodriguez B, Yan RS, Rafique S, Zhu MD, Li W, Liang XL, Gundlach D, Protasenko V, Kelly MM, Jena D, Liu L, Xing HG (2012) Extraordinary control of terahertz beam reflectance in graphene electro-absorption modulators. Nano Lett 12:4518–4522
Jadidi MM, Sushkov AB, Myers-Ward RL, Boyd AK, Daniels KM, Gaskill DK, Fuhrer MS, Drew HD, Murphy TE (2015) Tunable terahertz hybrid metal-graphene plasmons. Nano Lett 15:7099–7104
Chatzakis I, Li Z, Benderskii AV, Cronin SB (2017) Broadband terahertz modulation in electrostatically-doped artificial trilayer graphene. Nanoscale 9:1721–1726
Zhao YT, Wu B, Huang BJ, Cheng Q (2017) Switchable broadband terahertz absorber/reflector enabled by hybrid graphene-gold metasurface. Opt Express 25:7161–7169
Chen X, Fan WH (2017) Study of the interaction between graphene and planar terahertz metamaterial with toroidal dipolar resonance. Opt Lett 42:2034–2037
Tang PR, Li J, Zhong SC, Zhai ZH, Zhu B, Du LH, Li ZR, Zhu LG (2019) Giant dual-mode graphene-based terahertz modulator enabled by Fabry-Perot assisted multiple reflection. Opt Lett 44:1630–1633
Shen NH, Tassin P, Koschny T, Soukoulis CM (2014) Comparison of gold- and graphene-based resonant nanostructures for terahertz metamaterials and an ultrathin graphene-based modulator. Phys Rev B 90:115437
Sun YW, Degl’innocenti R, Ritchie DA, Beere HE, Xiao L, Ruggiero M, Zeitler JA, Stantchev RI, Chen D, Peng ZC, Macpherson E, Liu XD (2018) Graphene-loaded metal wire grating for deep and broadband THz modulation in total internal reflection geometry. Photonics Res 6:1151–1157
Liu ZZ, Zy L, Aydin K (2016) Time-varying metasurfaces based on graphene microribbon arrays. ACS Photonics 3:2035–2039
Yatooshi T, Ishikawa A, Tsuruta K (2015) Terahertz wavefront control by tunable metasurface made of graphene ribbons. Appl Phys Lett 107:053105
Zhang Z, Yan X, Liang LJ, Wei DQ, Wang M, Wang YR, Yao JQ (2018) The novel hybrid metal-graphene metasurfaces for broadband focusing and beam-steering in farfield at the terahertz frequencies. Carbon 132:529–538
Gao WL, Shu J, Reichel K, Nickel DV, He XW, Shi G, Vajtai R, Ajayan PM, Kono J, Mittleman DM, Xu QF (2014) High-contrast terahertz wave modulation by gated graphene enhanced by extraordinary transmission through ring apertures. Nano Lett 14:1242–1248
Lee SH, Choi M, Kim TT, Lee S, Liu M, Yin XB, Choi HK, Lee SS, Choi CG, Choi SY, Zhang X, Min B (2012) Switching terahertz waves with gate-controlled active graphene metamaterials. Nat Mater 11:936–941
Miao ZQ, Wu Q, Li X, He Q, Ding K, An ZH, Zhang YB, Zhou L (2015) Widely tunable terahertz phase modulation with gate-controlled graphene metasurfaces. Phys Rev X 5:041027
Zhang Y, Feng YJ, Zhao JM, Jiang T, Zhu B (2017) Terahertz beam switching by electrical control of graphene-enabled tunable metasurface. Sci Rep 7:14147
Zhang Y, Feng YJ, Jiang T, Cao J, Zhao JM, Zhu B (2018) Tunable broadband polarization rotator in terahertz frequency based on graphene metamaterials. Carbon 133:170–175
Zhang Y, Feng YJ, Zhu B, Zhao JM, Jiang T (2014) Graphene based tunable metamaterial absorber and polarization modulation in terahertz frequency. Opt Express 22:22743–22752
Zhang Y, Feng YJ, Zhu B, Zhao JM, Jiang T (2015) Switchable quarter-wave plate with graphene based metamaterial for broadband terahertz wave manipulation. Opt Express 23:27230–27239
Gao X, Yang WL, Cao WP, Chen M, Jiang YN, Yu XH, Li HO (2017) Bandwidth broadening of a graphene-based circular polarization converter by phase compensation. Opt Express 25:23945–23954
Kim TT, Oh SS, Kim HD, Park HS, Hess O, Min B, Zhang S (2017) Electrical access to critical coupling of circularly polarized waves in graphene chiral metamaterials. Sci Adv 3:e1701377
Zhu WR, Rukhlenko ID, Premaratne M (2013) Graphene metamaterial for optical reflection modulation. Appl Phys Lett 102:241914
Cheng H, Chen SQ, Yu P, Duan XY, Xie BY, Tian JG (2013) Dynamically tunable plasmonically induced transparency in periodically patterned graphene nanostrips. Appl Phys Lett 103:203112
Li L, Zhao H, Zhang JW (2017) Electrically tuning reflection of graphene-based Tamm plasmon polariton structures at 1550 nm. Appl Phys Lett 111:083504
Li DM, Wang W, Zhang H, Zhu YH, Zhang S, Zhang ZY, Zhang XP, Yi JM, Wei W (2018) Graphene-induced modulation effects on magnetic plasmon in multilayer metal-dielectric-metal metamaterials. Appl Phys Lett 112:131101
Habib M, Gokbayrak M, Ozbay E, Caglayan H (2018) Electrically controllable plasmon induced reflectance in hybrid metamaterials. Appl Phys Lett 113:221105
Khromova I, Andryieuski A, Lavrinenko A (2014) Ultrasensitive terahertz/infrared waveguide modulators based on multilayer graphene metamaterials. Laser Photonics Rev 8:916–923
He XY, Lu HX (2014) Graphene-supported tunable extraordinary transmission. Nanotechnology 25:325201
Kim S, Jang MS, Brar VW, Tolstova Y, Mauser KW, Atwater HA (2016) Electronically tunable extraordinary optical transmission in graphene plasmonic ribbons coupled to subwavelength metallic slit arrays. Nat Commun 7:12323
Yao Y, Kats MA, Genevet P, Yu NF, Song Y, Kong J, Capasso F (2013) Broad electrical tuning of graphene-loaded plasmonic antennas. Nano Lett 13:1257–1264
Youngblood N, Anugrah Y, Ma R, Koester SJ, Li M (2014) Multifunctional graphene optical modulator and photodetector integrated on silicon waveguides. Nano Lett 14:2741–2746
Gao YD, Shiue RJ, Gan XT, Li LZ, Peng C, Meric I, Wang L, Szep A, Walker D, Hone J, Englund D (2015) High-speed electro-optic modulator integrated with graphene-boron nitride heterostructure and photonic crystal nanocavity. Nano Lett 15:2001–2005
Thackray BD, Thomas PA, Auton GH, Rodriguez FJ, Marshall OP, Kravets VG, Grigorenko AN (2015) Super-narrow, extremely high quality collective plasmon resonances at telecom wavelengths and their application in a hybrid graphene-plasmonic modulator. Nano Lett 15:3519–3523
Kim S, Jang MS, Brar VW, Mauser KW, Kim L, Atwater HA (2018) Electronically tunable perfect absorption in graphene. Nano Lett 18:971–979
Kim Y, Kwon MS (2017) Mid-infrared subwavelength modulator based on grating-assisted coupling of a hybrid plasmonic waveguide mode to a graphene plasmon. Nanoscale 9:17429–17438
Argyropoulos C (2015) Enhanced transmission modulation based on dielectric metasurfaces loaded with graphene. Opt Express 23:23787–23797
Sun TB, Kim J, Yuk JM, Zettl A, Wang F, Chang-Hasnain C (2016) Surface-normal electro-optic spatial light modulator using graphene integrated on a high-contrast grating resonator. Opt Express 24:26035–26043
Aznakayeva DE, Rodriguez FJ, Marshall OP, Grigorenko AN (2017) Graphene light modulators working at near-infrared wavelengths. Opt Express 25:10255–10260
Liu GD, Zhai X, Xia SX, Lin Q, Zhao CJ, Wang LL (2017) Toroidal resonance based optical modulator employing hybrid graphene-dielectric metasurface. Opt Express 25:26045–26054
Huang BH, Lu WB, Liu ZG, Gao SP (2018) Low-energy high-speed plasmonic enhanced modulator using graphene. Opt Express 26:7358–7367
Vasić B, Gajić R (2014) Tunable Fabry-Perot resonators with embedded graphene from terahertz to near-infrared frequencies. Opt Lett 39:6253–6256
He XY, Zhao ZY, Shi WZ (2015) Graphene-supported tunable near-IR metamaterials. Opt Lett 40:178–181
Kim M, Jeong CY, Heo H, Kim S (2015) Optical reflection modulation using surface plasmon resonance in a graphene-embedded hybrid plasmonic waveguide at an optical communication wavelength. Opt Lett 40:871–874
Wang YL, Li T, Zhu SN (2017) Graphene-based plasmonic modulator on a groove-structured metasurface. Opt Lett 42:2247–2250
Tran TQ, Lee S, Heo H, Kim S (2016) Tunable wide-angle tunneling in graphene-assisted frustrated total internal reflection. Sci Rep 6:19975
Li ZY, Yu NF (2013) Modulation of mid-infrared light using graphene-metal plasmonic antennas. Appl Phys Lett 102:131108
Yao Y, Shankar R, Kats MA, Song Y, Kong J, Loncar M, Capasso F (2014) Electrically tunable metasurface perfect absorbers for ultrathin mid-infrared optical modulators. Nano Lett 14:6526–6532
Sherrott MC, Hon PWC, Fountaine KT, Garcia JC, Ponti SM, Brar VW, Sweatlock LA, Atwater HA (2017) Experimental demonstration of >230° phase modulation in gate-tunable graphene-gold reconfigurable mid-infrared metasurfaces. Nano Lett 17:3027–3034
Sorianello V, Midrio M, Contestabile G, Asselberghs I, Campenhout JV, Huyghebaert C, Goykhman I, Ott AK, Ferrari AC, Romagnoli M (2018) Graphene-silicon phase modulators with gigahertz bandwidth. Nat Photonics 12:40–44
Jang MS, Kim S, Brar VW, Menabde SG, Atwater HA (2018) Modulated resonant transmission of graphene plasmons across a λ/50 plasmonic waveguide gap. Phys Rev Appl 10:054053
Fu T, Chen YY, Wang TK, Li H, Zhang ZY, Wang L (2017) Active control of optical chirality with graphene-based achiral nanorings. Opt Express 25:24623–24629
Zhou SE, Lai PT, Dong GH, Li P, Li YX, Zhu Z, Guan CY, Shi JH (2019) Tunable chiroptical response of graphene achiral metamaterials in mid-infrared regime. Opt. Express 27:15359–15367
Owiti EO, Yang HN, Liu P, Ominde CF, Sun XD (2018) Polarization converter with controllable birefringence based on hybrid all-dielectric-graphene metasurface. Nanoscale Res Lett 13:38
Polat EO, Kocabas C (2013) Broadband optical modulators based on graphene supercapacitors. Nano Lett 13:5851–5857
Yu RW, Pruneri V, García de Abajo FJ (2015) Resonant visible light modulation with graphene. ACS Photonics 2:550–558
Yu RW, Pruneri V, García de Abajo FJ (2016) Active modulation of visible light with graphene-loaded ultrathin metal plasmonic antennas. Sci Rep 6:32144
Jiang XQ, Bao JL, Sun XD (2018) Multiwavelength optical switch based on controlling the Fermi energy of graphene. Phys Rev Appl 9:044026
Chu QQ, Song ZY, Liu QH (2018) Omnidirectional tunable terahertz analog of electromagnetically induced transparency realized by isotropic vanadium dioxide metasurfaces. Appl Phys Express 11:082203
Chen Y, Yao J, Song ZY, Ye LF, Cai GX, Liu QH (2016) Independent tuning of double plasmonic waves in a free-standing graphene-spacer-grating -spacer-graphene hybrid slab. Opt Express 24:16961–16972
Song ZY, Deng Y, Zhou YG, Liu ZY (2019) Terahertz toroidal metamaterial with tunable properties. Opt Express 27:5792–5797
Wang WH, Song ZY (2017) Multipole plasmons in graphene nanoellipses. Phys B 530:142–146
Watts CM, Liu XL, Padilla WJ (2012) Metamaterial electromagnetic wave absorbers. Adv Mater 24:OP98–OP120
Cui YX, He YR, Jin Y, Ding F, Yang L, Ye YQ, Zhong SM, Lin YY, He SL (2014) Plasmonic and metamaterial structures as electromagnetic absorbers. Laser Photonics Rev 8:495–520
Wei ML, Song ZY, Deng Y, Liu YN, Chen Q (2019) Large-angle mid-infrared absorption switch enabled by polarization-independent GST metasurfaces. Mater Lett 236:350–353
Song ZY, Chen AP, Zhang J, Wang JY (2019) Integrated metamaterial with functionalities of absorption and electromagnetically induced transparency. Opt Express 27:25196–25204
Tang CJ, Yan ZD, Wang QG, Chen J, Zhu MW, Liu B, Liu FX, Sui CH (2015) Ultrathin amorphous silicon thin-film solar cells by magnetic plasmonic metamaterial absorbers. RSC Adv 5:81866–81874
Liu B, Tang CJ, Chen J, Xie NY, Tang H, Zhu XQ, Park GS (2018) Multiband and broadband absorption enhancement of monolayer graphene at optical frequencies from multiple magnetic dipole resonances in metamaterial. Nanoscale Res Lett 13:153
Liu B, Tang CJ, Chen J, Wang QG, Pei MX, Tang H (2017) Dual-band light absorption enhancement of monolayer graphene from surface plasmon polaritons and magnetic dipole resonances in metamaterials. Opt Express 25:12061–12068
Johnson PB, Christy RW (1972) Optical constants of the noble metals. Phys Rev B 6:4370–4379
Xiang YJ, Guo J, Dai XY, Wen SC, Tang DY (2014) Engineered surface Bloch waves in graphene-based hyperbolic metamaterials. Opt Express 22:3054–3062
Ghamsari BG, Olivieri A, Variola F, Berini P (2014) Enhanced Raman scattering in graphene by plasmonic resonant Stokes emission. Nanophotonics 3:363–371
Sun S, Yi NB, Yao WJ, Song QH, Xiao SM (2014) Enhanced second-harmonic generation from nonlinear optical metamagnetics. Opt Express 22:26613–26620
This work is financially supported by the National Natural Science Foundation of China (NSFC) under Grant Nos. 11974188, 11704183, 61405134, 61340007, 11304159, and 11104136; PAPD; NSFJS under Grant No. BK20161512; NSFZJ under Grant No. LY14A040004; China Postdoctoral Science Foundation under Grant No. 2018 M632345; Qing Lan Project of Jiangsu Province; Open Project of State Key Laboratory of Millimeter Waves under Grant No. K201821; NUPTSF under Grant Nos. NY218022 and NY217045.
Ethics Approval and Consent to Participate
We declare that there are no concerning data of human and animals.
The authors declare that they have no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
About this article
Cite this article
Ji, Y., Yan, Z., Tang, C. et al. Efficient Optical Reflection Modulation by Coupling Interband Transition of Graphene to Magnetic Resonance in Metamaterials. Nanoscale Res Lett 14, 391 (2019). https://doi.org/10.1186/s11671-019-3233-2
- Reflection modulation
- Magnetic resonance